Crash and Impact Simulation of Composite Structures by Using CAE Process Chain

 Leon Griffin
 5 months ago
 Views:
Transcription
1 Crash and Impact Simulation of Composite Structures by Using CAE Process Chain Madhukar Chatiri 1, Thorsten Schütz 2, Anton Matzenmiller 3, Ulrich Stelzmann 1 1 CADFEM GmbH, Grafing/Munich, Germany, 2 Adam Opel AG, GME Vehicle CAE, Ruesselsheim, Germany, 3 Dept. of Mech. Engineering, Univ. of Kassel, Kassel, Germany, Abstract The objective of this paper is to present a workflow for numerical modeling and simulation of carbon fiber reinforced plastic (CFRP) composite structures including CAE process integration. A computational constitutive model for anisotropic damage is developed to characterize the elasticbrittle behavior of fiberreinforced laminated composites. The composite damage model is implemented within LSDYNA as user defined material subroutine. A CAE process chain which includes the manufacturing side of composites is also presented. Keywords: CFRP, CAE process chain 11
2 Session: Simulation 13 th International LSDYNA Users Conference 1 Introduction The challenging demands of the automotive industry include increased global competition, the need for vehicles with highest efficiency, a reduction in costs and stringent environmental and safety requirements. The materials used in automotive engineering play key roles in overcoming these challenges and eventually lighter materials mean lighter vehicles and low greenhouse gas emissions. Composites are being used increasingly in the automotive industry due to their strength, quality and light weight. In the present work, a CAE process chain is described which consists of the following parts:  Virtual vessel generation using ANSYS Composite PrepPost for thick walled composite structures  3D explicit FEA of the composite vessel with (a) Multilayered solid elements and (b) constitutive model wherein the damage initiation criteria are based on Puck failure criterion for first ply failure and progressive micro crack propagation is based on the idea of continuum damage evolution. The adaptation to thin walled composite structures is also discussed in the end. 2 CAE process chain In this section, the CAE tool chain is explained for high pressure hydrogen storage system (HSS) for fuel cell vehicles with an operating pressure of 70 MPa manufactured of carbon fiber reinforced plastic (CFRP) material. Here, three aspects are important. Firstly, the vessel has to fit into the given package space of the vehicle. Secondly, the vessel has to withstand a certain inner pressure and third, the vessel plus integration features have to pass certain vehicle crash acceptance criteria. Thus it is necessary to integrate the high pressure vessel into standard CAE processes in order to work on these aspects in the early phase of a fuel cell vehicle development. The aspect of data importing/exporting interface between individual tools, especially between the wetwinding process simulation and the FEA tools is quite efficiently done in the current tool chain (see Fig. 2.1). Starting point in the vessel predimensioning phase is the given package envelope of the vehicle. This envelope defines the maximum outer dimensions of the vessel at maximum allowable working pressure. In the next step the nominal outer dimensions of the vessel are determined using an estimation of the expansion of the vessel under pressure. An iterative process is applied to determine the required number of helical and hoop layers, the starting winding angle and the thickness of the composite. The whole iterative process considers just the cylindrical part of the vessel assuming a two dimensional state of stress and applies netting theory and classical laminate theory in a subsequent manner. In the next step, a detailed geometrical representation of the fiber layup inside the wall of a composite vessel is developed by using inhouse tool Pywind. Each unidirectional (UD) layer of a composite pressure vessel is considered individually with respect to its winding angle, fiber properties and coefficient of friction. 12
3 In the third step, the Pywind data is imported inside ANSYS Composite PrepPost (ACP) and a detailed FE mesh of the wet wound composite vessel is generated. The output of the FE mesh is *ELEMENT_TSHELL_COMPOSITE [1] which allows a very comfortable description of composite layers using a plybased concept. The FE solid model consists of a Multilayered solid element (TSHELL type 5) which resolves the 3D stress state necessary for impact directions normal to the outer vessel surface. Also this element allows the definition of multiple integration points through the thickness in order to account for stacks of plies with arbitrary fiber orientation. In the final step, Impact and crash simulation models are generated inside LSPrePost and simulations are done using LSDYNA. Fig. 2.1 CAE process chain for thick walled composite structures 3 Constitutive modeling A computational constitutive model for anisotropic damage is developed to characterize the elasticbrittle behavior of fiberreinforced laminated composites. The composite damage model is implemented within LSDYNA as user defined material subroutine which can describe progressive failure and damage behavior of carbon fiber reinforced plastic (CFRP) composites. A homogenized continuum is adopted for the constitutive theory of anisotropic damage and elasticity. Damage initiation criteria or first ply failure prediction is based on Puck failure criterion and progressive damage is based on continuum damage mechanics. Internal variables are introduced to describe the evolution of the damage state under loading and as a consequence the degradation of the material stiffness occurs. The corresponding rate equations are subjected to laws of thermomechanics. Emphasis is placed on a suitable coupling among the equations for the rates of the damage variables with respect to different damage modes. The integrated routine is successfully utilized to predict failure and damage of composite laminates which are subjected to impact conditions. 3.1 Fibre failure (FF) or longitudinal failure Stresses in fibre direction are predominantly transmitted through the fibres because of their high stiffness and strength in comparison with the properties of the matrix material. The transmission 13
4 Session: Simulation 13 th International LSDYNA Users Conference of tensile stresses in the fibres is hardly impaired by the state of damage in the matrix, since fibres straighten under high tension. The straightening of the fibres may contribute to matrix damage in the absence of fibre rupture. The load carrying capacity of fibres in compression, however, is severely affected by the effective stiffness and strength of the surrounding matrix phase. The matrix acts like an "elastic foundation" for the fibres, treated in mechanical models as beams under compression. Both, fibre rupture due to tension, and buckling or kinking of fibres due to compression cause damage evolution in resin matrices. As a consequence, all stiffness components of the constitutive tensor for the damaged unidirectional lamina are typically degraded. As explained above, fibre fracture is primarily caused by the stress which acts parallel to the fibres. It expresses the physical idea that fibre fracture under a multiaxial state of stress in a UDlamina occurs when its stress parallel to the fibres is equal to or exceeds the stress necessary for fracture. The simple Puck FFcondition follows from this hypothesis [2, 3, and 4]. It describes by case distinction the tensile fibre mode, for 0: = 1 and the compressive fibre mode for <0:, = 1 wherein, denote the corresponding material strength parameters. 3.2 Interfibre failure (IFF) or transverse failure Normal stresses, acting transverse to the fibres and shear stresses are transmitted through both matrix and fibres. However, their damaging effect mainly takes place in the matrix or in the fibrematrix interface, leading to debonding. Usually, the bond strength of the interface zone between fibres and matrix is the lowest in comparison to the data for the strength of the single constituents. Advancing cracks in the matrix soon pass into the fibrematrix interface and propagate along the fibres without crossing into the fibre material. Progressive opening of existing cracks is characteristic for tensile loading in transverse direction, whereas "crushing" in the sense of "fragmentation" of brittle matrix materials is very typical for compression in transverse direction. Following the FF, see Fig. 3.1 a, 3.1 b and IFF, see Fig. 3.1 c, 3.1 d, 3.1 e, observations outlined above, the failure modes considered in the model proposed here are schematically represented in Fig (1) (2) Fig. 3.1: Major failure modes considered in the model as in Knops (2008) 14
5 For the above described transverse failure, the Puck IFF criteria are most promising for brittle, plastic unidirectional (UD) laminates  see Fig The UDply behaves transversely isotropic in both cases, elasticity and failure. Puck assumes a Mohr Coulomb type of failure criterion for loading transverse to the fibre direction. Failure is assumed to be caused by the normal and shear components operating on the action plane of stresses,,  see Fig Positive normal stress on this plane promotes fracture while a negative one increases the material s shear strength, thus, impeding fracture. Puck s stress based failure criteria enable the computation of the material exposure f, () as a failure indicator, wherein is the orientation angle. Figure 3.2: Schematic representation of failure modes and failure plane based on Puck, as in [3] The 3D Puck failure criterion can be categorized as below in Tab. 1 in extension to Fig. 3.2 Table 1: Categorization of fracture modes in failure criteria of Puck under three dimensional stress states Fracture angle Sign of Fracture mode 90 positive Delamination 0 to 89 positive A 53 to 0 negative B 90 to 53 negative C The values of f, () range between 0, where the material is unstressed, and up to 1, denoting the onset of IFF. The master failure surface on the fracture plane is defined in terms of the Mohr Coulomb stresses, thus, yielding the following failure criteria by case distinction in tension and compression: for 0:, () = and () + () + () + () 1 (3) 15
6 Session: Simulation 13 th International LSDYNA Users Conference for <0:, 16 () = () + () + () + () 1 (4) The only unknown parameters in these equations are ±,, and which depend on the shear stresses and according to the following equations: ± and = ± = + ± (5) ±, wherein,, denote the corresponding material strength parameters, and ± are constants introduced by Puck, see [4]. The action plane with the greatest failure effort () (wherein = ) is the fracture plane to be expected, () =. Once the failure plane with max () is found, the fracture angle as is kept constant in the model and progressive failure, based on the idea of continuum damage, is applied to the material model for the corresponding lamina at hand, see below. The failure criteria may be interpreted as loading criteria, a terminology encountered in strain space plasticity. The role played by the yield stress in plasticity will be taken by the threshold variables in damage mechanics. In classical continuum damage mechanics, only the undamaged (whole) part of the crosssection (netarea) for the uniaxial case is supposed to carry loading, i.e. transmit stresses. Consequently, the stresses in the failure criteria should be interpreted as effective stresses, referred to the net area. This means that the failure criteria are assumed to hold in terms of the effective stresses rather than the nominal ones. If the degradation is described in the sense of CAUCHY s stress concept, six different nonnegative damage parameters,,,, and are defined to quantify the relative size of macro cracks projected onto the coordinate planes, and assembled in the rankfour damage operator given in VOIGT notation of Eq. 8d. In CDM, the effective normal stresses are related to the damage parameters ω, since only the undamaged part of the cross section for the uniaxial case is supposed to carry loading. Consequently, the stresses in the failure criteria should be interpreted as effective stresses, referred to the net area. A simple relationship between effective stress and the nominal one holds: = (7) wherein represents the rankfour (uncoupled) damage operator given in VOIGT notation as: 0 0 = 0 0, =, = 0 0, = (6) (8ad)
7 In the undamaged state, a lamina behaves equally in the transverse 2direction and the throughthickness 3direction which allows to reduce the general anisotropy to a transversely isotropic behavior with only a fibreparallel (1) and fibreperpendicular (2) direction. The constitutive behavior, i.e. the material equation relating, states of stress to states of strain, is then defined by the transversely isotropic compliance matrix in VOIGT notation for the UDlaminae prior to the damage initiation, see Eq. 9. Only the inplane shear modulus ( ) is modelled. 2 = ( ) (9) The components of the constitutive tensor are represented as functions of the vector, comprising all internal damage variables, and the material parameters of the undamaged lamina. The constitutive tensor ()is derived by physical arguments and information of the dependencies between effective elastic properties and individual damage variables. Generally, for a given arbitrary damage operator, the postulate of strain equivalence yields an unsymmetrical constitutive tensor, which should be rejected as a model for the elastic behavior. This hypothesis serves here as a first guidance together with physical arguments to set up the constitutive tensor () for the damaged lamina. For the purpose of building the dependence on damage into the constitutive assumption, the compliance relationship is more easily accessible in order to relate the material parameters to the mechanical response in the coordinate system with preferred axes. The compliance relationship for orthotropic elasticity in terms of effective stresses reads as: =, = ( ) 0 0 0, = It is to be noted that Eq. (10b) is symmetric. Equations (7) and (10a) result in: = = (10ac) The final relationship of the compliance tensor for the damaged laminae () takes the following form after POISSON s ratios () and () are adjusted according to the qualitative arguments presented in [5]. (11) 17
8 Session: Simulation 13 th International LSDYNA Users Conference () = ( ) ( ) ( ) ( ) ( 12 ) ( ) 0 ( ) (12) As explained earlier, the orthotropic nature of the lamina as a homogenized continuum is maintained throughout the damaging process. The shear coupling terms are neglected. Therefore, the symmetry class of the UDlamina remains the same for all states of damage. Its inverse always exits as long as the damage variables are less than one ( <1). Hence, the material stiffness tensor is given by: () = () 3.3 Verification example In this verification example, a tension test under loading transverse to fibre direction on a UDreinforced laminated composite is presented. The lamina material properties for elasticity are: =126GPa, =11GPa, =11GPa, =0.28, =0.40, =0.28, =9GPa; and for strength: () = 45 MPa, = 79MPa, () = 1950 MPa. The load is applied in transverse (to fibre) direction until complete failure. Fig. 3.3 left and Fig. 3.3 right represents the evolution of damage variables in both original two dimensional (2D) model and the current three dimensional (3D) extension of the model for strain softening exponent =1.0. Unlike in the original two dimensional model from [5], where the damage variables effect the stressstrain curves over the entire strain range, in the current model, the damage variables are only applicable to the postfailure part. Figure 3.3: left: Evolution of damage variable in the original 2D model and current 3D model and right: transverse stressstrain curve in both the models 18
9 3.4 Comparison with other material models inside LSDYNA The current userdefined material model is also tested and compared with the available material models within LSDYNA, see Fig Figure 3.4: Comparison of stresses with material models within LSDYNA 3.5 Validation example A 4point bending response on a laminate with configuration of (±20 2 /90 4 /±20 2 /90 4 ) is shown in the below example. The material properties are taken from OPEL. The simulated model is a quarter symmetry model. Fig. 3.5 (left) shows the IFF predicted by Puck failure criteria and Fig. 3.5 (right) shows the force vs. strain results compared with experiment. 19
10 Session: Simulation 13 th International LSDYNA Users Conference Figure 3.5: left: Firsply failure (IFF) inside the tube using 3D puck failure criteria and right: comparison with test (strain gauge signal from tension side) 4 Adaptation to thin shell structures The CAE process chain which is developed for thick composite structures is adapted to thin shell structures. The thin shell composite draping simulation is done using FiberSim and this data is imported inside ACP to build the composite shell structure (see Fig. 4.1). The output of the FE mesh is *ELEMENT_SHELL_COMPOSITE [1] which allows a very comfortable description of composite layers using a plybased concept. Also the three dimensional material model is adapted to thin shell structures. 110
11 Fig. 4.1 CAE process chain for thin shell composite structures 5 Summary and conclusions The CAE process chain is successfully implemented in the design phase both for thick as well as thin composite structures. The mesolevel model with the 3D Puck failure criteria and anisotropic continuum damage mechanics is very effective in analyzing multilayered structures having a large number of plies. The developed material model describes both onset and progression of damage. It can reproduce the key physical aspects observed in the failure of Fibrereinforced laminated composites. 6 References [1] Hallquist, J.O.: LSDYNA Keyword Manual Version 971. Livermore Software Technology Corporation, Livermore, 2013 [2] Hashin, Z. : Failure criteria for unidirectional fibre composites, J. Appl. Mech. vol. 47, pp , 1980 [3] Knops, M.: Analysis of Failure in Fibre Polymer Laminates: The Theory of Alfred Puck. Springer Verlag: Berlin, Heidelberg, 2008 [4] Puck, A.; Schürmann, H. : Failure analysis of FRP laminates by means of physically based phenomenological models, in Failure Criteria in Fibre Reinforced Polymer Composites: The World Wide Failure Exercise, P. D. Hinton, A. S. Kaddour, and M. L. Soden, Eds. Elsevier: Oxford, pp , 2004 [5] Matzenmiller, A.; Lubliner, J.; Taylor, R. L.: A constitutive model for anisotropic damage in fibre composites, Mechanics of Materials, vol. 20, pp ,
QUESTION BANK Composite Materials
QUESTION BANK Composite Materials 1. Define composite material. 2. What is the need for composite material? 3. Mention important characterits of composite material 4. Give examples for fiber material 5.
More informationNumerical simulation of delamination onset and growth in laminated composites
Numerical simulation of delamination onset and growth in laminated composites G. Wimmer, C. Schuecker, H.E. Pettermann Austrian Aeronautics Research (AAR) / Network for Materials and Engineering at the
More informationISSN: ISO 9001:2008 Certified International Journal of Engineering Science and Innovative Technology (IJESIT) Volume 2, Issue 4, July 2013
Delamination Studies in FibreReinforced Polymer Composites K.Kantha Rao, Dr P. Shailesh, K. Vijay Kumar 1 Associate Professor, Narasimha Reddy Engineering College Hyderabad. 2 Professor, St. Peter s Engineering
More informationTensile behaviour of antisymmetric CFRP composite
Available online at www.sciencedirect.com Procedia Engineering 1 (211) 1865 187 ICM11 Tensile behaviour of antisymmetric CFRP composite K. J. Wong a,b, *, X. J. Gong a, S. Aivazzadeh a, M. N. Tamin b
More informationLAMINATION THEORY FOR THE STRENGTH OF FIBER COMPOSITE MATERIALS
XXII. LAMINATION THEORY FOR THE STRENGTH OF FIBER COMPOSITE MATERIALS Introduction The lamination theory for the elastic stiffness of fiber composite materials is the backbone of the entire field, it holds
More informationDESIGN OF LAMINATES FOR INPLANE LOADING
DESIGN OF LAMINATES FOR INPLANOADING G. VERCHERY ISMANS 44 avenue F.A. Bartholdi, 72000 Le Mans, France Georges.Verchery@m4x.org SUMMARY This work relates to the design of laminated structures primarily
More informationBIAXIAL STRENGTH INVESTIGATION OF CFRP COMPOSITE LAMINATES BY USING CRUCIFORM SPECIMENS
BIAXIAL STRENGTH INVESTIGATION OF CFRP COMPOSITE LAMINATES BY USING CRUCIFORM SPECIMENS H. Kumazawa and T. Takatoya Airframes and Structures Group, Japan Aerospace Exploration Agency 6131, Ohsawa, Mitaka,
More informationComposite Materials 261 and 262
Composite Materials 261 and 262 Stefan Hartmann 1 David Moncayo 2 1 DYNAmore GmbH, Stuttgart, Germany 2 Daimler AG, Sindelfingen, Germany 11. LSDYNA Forum 2012, 9.  10. Oktober 2012, Ulm 1 Outline Introduction
More informationS. Srinivasan, Technip Offshore, Inc., Houston, TX
9 th ASCE Specialty Conerence on Probabilistic Mechanics and Structural Reliability PROBABILISTIC FAILURE PREDICTION OF FILAMENTWOUND GLASSFIBER Abstract REINFORCED COMPOSITE TUBES UNDER BIAXIAL LOADING
More informationAn investigation of the mechanical behaviour of carbon epoxy cross ply cruciform specimens under biaxial loading
An investigation of the mechanical behaviour of carbon epoxy cross ply cruciform specimens under biaxial loading A. Makris, C. Ramault, D. Van Hemelrijck Department of Mechanics of Materials and Constructions,
More informationEnhancing Prediction Accuracy In Sift Theory
18 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS Enhancing Prediction Accuracy In Sift Theory J. Wang 1 *, W. K. Chiu 1 Defence Science and Technology Organisation, Fishermans Bend, Australia, Department
More informationMECHANICS OF MATERIALS. EQUATIONS AND THEOREMS
1 MECHANICS OF MATERIALS. EQUATIONS AND THEOREMS Version 20110114 Stress tensor Definition of traction vector (1) Cauchy theorem (2) Equilibrium (3) Invariants (4) (5) (6) or, written in terms of principal
More informationFinite element modelling of infinitely wide Angleply FRP. laminates
www.ijaser.com 2012 by the authors Licensee IJASER Under Creative Commons License 3.0 editorial@ijaser.com Research article ISSN 2277 9442 Finite element modelling of infinitely wide Angleply FRP laminates
More informationITE IMPACT ON. Summary. concurrent. phenomena delamination. subroutine. simulations discussed. Keywords: Volnei Tita.
NUMERICAL AND EXPERIMENTAL ANALYSES OF LOW VELOCITY IMPACT ON THIN COMPOS ITE Marcelo L. Ribeiro Department of Aeronautical Engineeringg Engineering Scholl of São Carlos University of São S Paulo malribei@usp.
More informationAnisotropic modeling of short fibers reinforced thermoplastics materials with LSDYNA
Anisotropic modeling of short fibers reinforced thermoplastics materials with LSDYNA Alexandre Hatt 1 1 Faurecia Automotive Seating, Simplified Limited Liability Company 1 Abstract / Summary Polymer thermoplastics
More informationModule 7: Micromechanics Lecture 29: Background of Concentric Cylinder Assemblage Model. Introduction. The Lecture Contains
Introduction In this lecture we are going to introduce a new micromechanics model to determine the fibrous composite effective properties in terms of properties of its individual phases. In this model
More informationA FINITE ELEMENT MODEL TO PREDICT MULTI AXIAL STRESSSTRAIN RESPONSE OF CERAMIC MATRIX COMPOSITES WITH STRAIN INDUCED DAMAGE
A FINITE ELEMENT MODEL TO PREDICT MULTI AXIAL STRESSSTRAIN RESPONSE OF CERAMIC MATRIX COMPOSITES WITH STRAIN INDUCED DAMAGE Daxu Zhang and D. R. Hayhurst School of Mechanical, Aerospace and Civil Engineering,
More information14. LSDYNA Forum 2016
14. LSDYNA Forum 2016 A Novel Approach to Model Laminated Glass R. Böhm, A. Haufe, A. Erhart DYNAmore GmbH Stuttgart 1 Content Introduction and Motivation Common approach to model laminated glass New
More information*MAT_PAPER and *MAT_COHESIVE_PAPER: Two New Models for Paperboard Materials
14 th International LSDYNA Users Conference Session: Constitutive Modeling *MAT_PAPER and *MAT_COHESIVE_PAPER: Two New Models for Paperboard Materials Jesper Karlsson 1, Mikael Schill 1, Johan Tryding
More informationMULTISCALE AND MULTILEVEL ANALYSIS OF COMPOSITE STRUCTURES WITH BOLTED JOINTS
MULTISCALE AND MULTILEVEL ANALYSIS OF COMPOSITE STRUCTURES WITH BOLTED JOINTS F.X. Irisarri, J.F. Maire* and N. Carrere ONERA, 9 av. de la Division Leclerc, 930 Châtillon, France francoisxavier.irisarri@onera.fr,
More informationTHE ROLE OF DELAMINATION IN NOTCHED AND UNNOTCHED TENSILE STRENGTH
THE ROLE OF DELAMINATION IN NOTCHED AND UNNOTCHED TENSILE STRENGTH M. R. Wisnom University of Bristol Advanced Composites Centre for Innovation and Science University Walk, Bristol BS8 1TR, UK M.Wisnom@bristol.ac.uk
More informationBUCKLING AND POSTBUCKLING IN FILAMENT WOUND COMPOSITE TUBES UNDER TRANSVERSE COMPRESSION
2 th International Conference on Composite Materials Copenhagen, 1924 th July 215 BUCKLING AND POSTBUCKLING IN FILAMENT WOUND COMPOSITE TUBES UNDER TRANSVERSE COMPRESSION José Humberto S. Almeida Jr.
More informationA synergistic damage mechanics approach to mechanical response of composite laminates with ply cracks
Article A synergistic damage mechanics approach to mechanical response of composite laminates with ply cracks JOURNAL OF COMPOSITE MATERIALS Journal of Composite Materials 0(0) 7! The Author(s) 0 Reprints
More informationREPRESENTING MATRIX CRACKS THROUGH DECOMPOSITION OF THE DEFORMATION GRADIENT TENSOR IN CONTINUUM DAMAGE MECHANICS METHODS
20 th International Conference on Composite Materials Copenhagen, 1924 th July 2015 REPRESENTING MATRIX CRACKS THROUGH DECOMPOSITION OF THE DEFORMATION GRADIENT TENSOR IN CONTINUUM DAMAGE MECHANICS METHODS
More informationMaterials and Structures. Indian Institute of Technology Kanpur
Introduction to Composite Materials and Structures Nachiketa Tiwari Indian Institute of Technology Kanpur Lecture 16 Behavior of Unidirectional Composites Lecture Overview Mt Material ilaxes in unidirectional
More informationEXPERIMENTAL AND NUMERICAL STUDY OF THE ENERGY ABSORPTION CAPACITY OF PULTRUDED COMPOSITE TUBES
EXPERIMENTAL AND NUMERICAL STUDY OF THE ENERGY ABSORPTION CAPACITY OF PULTRUDED COMPOSITE TUBES D. Kakogiannis 1, D. Van Hemelrijck 1, J. Wastiels 1, S. Palanivelu 2, W. Van Paepegem 2, K. De Wolf 3, J.
More informationEVALUATION OF DAMAGE DEVELOPMENT FOR NCF COMPOSITES WITH A CIRCULAR HOLE BASED ON MULTISCALE ANALYSIS
THE 19 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS EVALUATION OF DAMAGE DEVELOPMENT FOR NCF COMPOSITES WITH A CIRCULAR HOLE BASED ON MULTISCALE ANALYSIS T. Kurashiki 1 *, Y. Matsushima 1, Y. Nakayasu
More informationMECHANICAL CHARACTERISTICS OF CARBON FIBER YACHT MASTS
MECHANICAL CHARACTERISTICS OF CARBON FIBER YACHT MASTS This paper provides a preliminary stress analysis of a carbon reinforced layered cylinder such as would be found in a yacht mast. The cylinder is
More informationNigerian Journal of Technology, Vol. 26, No. 2, June 2007 Edelugo 37
Nigerian Journal of Technology, Vol. 26, No. 2, June 2007 Edelugo 37 APPLICATION OF THE REISSNERS PLATE THEORY IN THE DELAMINATION ANALYSIS OF A THREEDIMENSIONAL, TIME DEPENDENT, NONLINEAR, UNIDIRECTIONAL
More informationVALIDATION of CoDA SOFTWARE for COMPOSITES SYNTHESIS AND PRELIMINARY DESIGN (or GETTING COMPOSITES USED  PART 2 )
VALIDATION of CoDA SOFTWARE for COMPOSITES SYNTHESIS AND PRELIMINARY DESIGN (or GETTING COMPOSITES USED  PART 2 ) Graham D Sims and William R Broughton Composites Design Data and Methods, Centre for Materials
More informationModeling Hailstone Impact onto Composite Material Panel Under a Multiaxial State of Stress
Modeling Hailstone Impact onto Composite Material Panel Under a Multiaxial State of Stress Authors Marco ANGHILERI * LuigiM L CASTELLETTI * Andrea MILANESE * and Andrea SEMBOLONI * Affiliation * Politecnico
More informationPrediction of Delamination Growth Behavior in a Carbon Fiber Composite Laminate Subjected to Constant Amplitude CompressionCompression Fatigue Loads
Prediction of Delamination Growth Behavior in a Carbon Fiber Composite Laminate Subjected to Constant Amplitude CompressionCompression Fatigue Loads J. Raju 1*, D.S. Sreedhar 2, & C.M. Manjunatha 1 1
More information6. NONLINEAR PSEUDOSTATIC ANALYSIS OF ADOBE WALLS
6. NONLINEAR PSEUDOSTATIC ANALYSIS OF ADOBE WALLS Blondet et al. [25] carried out a cyclic test on an adobe wall to reproduce its seismic response and damage pattern under inplane loads. The displacement
More information*Corresponding author: Keywords: Finiteelement analysis; Multiscale modelling; Onset theory; Dilatational strain invariant.
18 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS MICROMECHANICAL MODELLING OF TEST SPECIMENS FOR ONSET OF DILATATIONAL DAMAGE OF POLYMER MATRIX IN COMPOSITE MATERIALS T. D. Tran 1, D. Kelly 1*, G.
More informationFracture Mechanics of Composites with Residual Thermal Stresses
J. A. Nairn Material Science & Engineering, University of Utah, Salt Lake City, Utah 84 Fracture Mechanics of Composites with Residual Thermal Stresses The problem of calculating the energy release rate
More informationBALLISTIC IMPACT MODELING OF COMPOSITE MATERIALS
7 th International LSDYNA Users Conference Penetration/Explosive BALLISTIC IMPACT MODELING OF COMPOSITE MATERIALS ChianFong Yen Materials Sciences Corporation 5 Office Center Drive Fort Washington, PA
More informationMechanics of Composite Materials, Second Edition Autar K Kaw University of South Florida, Tampa, USA
Mechanics of Composite Materials, Second Edition Autar K Kaw University of South Florida, Tampa, USA What programs are in PROMAL? Master Menu The master menu screen with five separate applications from
More informationLecture #10: Anisotropic plasticity Crashworthiness Basics of shell elements
Lecture #10: 1510735: Dynamic behavior of materials and structures Anisotropic plasticity Crashworthiness Basics of shell elements by Dirk Mohr ETH Zurich, Department of Mechanical and Process Engineering,
More informationPlane Strain Test for Metal Sheet Characterization
Plane Strain Test for Metal Sheet Characterization Paulo Flores 1, Felix Bonnet 2 and AnneMarie Habraken 3 1 DIM, University of Concepción, Edmundo Larenas 270, Concepción, Chile 2 ENS  Cachan, Avenue
More informationTuesday, February 11, Chapter 3. Load and Stress Analysis. Dr. Mohammad Suliman Abuhaiba, PE
1 Chapter 3 Load and Stress Analysis 2 Chapter Outline Equilibrium & FreeBody Diagrams Shear Force and Bending Moments in Beams Singularity Functions Stress Cartesian Stress Components Mohr s Circle for
More informationME 582 Advanced Materials Science. Chapter 2 Macromechanical Analysis of a Lamina (Part 2)
ME 582 Advanced Materials Science Chapter 2 Macromechanical Analysis of a Lamina (Part 2) Laboratory for Composite Materials Research Department of Mechanical Engineering University of South Alabama, Mobile,
More informationChapter 3. Load and Stress Analysis
Chapter 3 Load and Stress Analysis 2 Shear Force and Bending Moments in Beams Internal shear force V & bending moment M must ensure equilibrium Fig. 3 2 Sign Conventions for Bending and Shear Fig. 3 3
More information3D Finite Element analysis of stud anchors with large head and embedment depth
3D Finite Element analysis of stud anchors with large head and embedment depth G. Periškić, J. Ožbolt & R. Eligehausen Institute for Construction Materials, University of Stuttgart, Stuttgart, Germany
More informationFINITE ELEMENT ANALYSIS OF A LAYERED COMPOSITE CYLINDER USING THE CONNECTION BETWEEN THE MACRO AND MICROSTRUCTURE
FINITE ELEMENT ANALYI OF A LAYERED COMPOITE CYLINDER UING THE CONNECTION BETWEEN THE MACRO AND MICROTRUCTURE A. zekrényes Research Assistant, Department of Applied Mechanics, Budapest University of Technology
More informationNonlinear Analysis of Reinforced Concrete Shells Subjected to Impact Loads
Transactions of the 7 th International Conference on Structural Mechanics in Reactor Technology (SMiRT 7) Prague, Czech Republic, August 7, 00 Paper # J0 Nonlinear Analysis of Reinforced Concrete Shells
More informationPRELIMINARY PREDICTION OF SPECIMEN PROPERTIES CLT and 1 st order FEM analyses
OPTIMAT BLADES Page 1 of 24 PRELIMINARY PREDICTION OF SPECIMEN PROPERTIES CLT and 1 st order FEM analyses first issue Peter Joosse CHANGE RECORD Issue/revision date pages Summary of changes draft 241002
More informationSOME RESEARCH ON FINITE ELEMENT ANALYSIS OF COMPOSITE MATERIALS
Mechanical Testing and Diagnosis ISSN 2247 9635, 2012 (II), Volume 3, 7985 SOME RESEARCH ON FINITE ELEMENT ANALYSIS OF COMPOSITE MATERIALS Valeriu DULGHERU, Viorel BOSTAN, Marin GUŢU Technical University
More informationFASTENER PULLTHROUGH FAILURE IN GFRP LAMINATES
18 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS FASTENER PULLTHROUGH FAILURE IN GFRP LAMINATES G. Catalanotti 1*, P.P. Camanho 1, P. Ghys 2, A.T. Marques 1 1 DEMec, Faculdade de Engenharia, Universidade
More informationAPPLICATION OF A SCALAR STRAINBASED DAMAGE ONSET THEORY TO THE FAILURE OF A COMPLEX COMPOSITE SPECIMEN
28 TH INTERNATIONAL CONGRESS OF THE AERONAUTICAL SCIENCES APPLICATION OF A SCALAR STRAINBASED DAMAGE ONSET THEORY TO THE FAILURE OF A COMPLEX COMPOSITE SPECIMEN Tuyen Tran*, Dan Simkins**, Shen Hin Lim*,
More informationSTRESS ANALYSIS OF A FILAMENT WOUND COMPOSITE FLYWHEEL DISK
THE 19 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS STRESS ANALYSIS OF A FILAMENT WOUND COMPOSITE FLYWHEEL DISK Md. S. Uddin 1*, E. V. Morozov 1 and K. Shankar 1 1 School of Engineering and Information
More information4.MECHANICAL PROPERTIES OF MATERIALS
4.MECHANICAL PROPERTIES OF MATERIALS The diagram representing the relation between stress and strain in a given material is an important characteristic of the material. To obtain the stressstrain diagram
More informationMODELING SLABCOLUMN CONNECTIONS REINFORCED WITH GFRP UNDER LOCALIZED IMPACT
MODELING SLABCOLUMN CONNECTIONS REINFORCED WITH GFRP UNDER LOCALIZED IMPACT QI ZHANG and AMGAD HUSSEIN Faculty of Engineering, Memorial University of Newfoundland St. John s, Newfoundland, Canada, A1B
More informationMicromeso draping modelling of noncrimp fabrics
Micromeso draping modelling of noncrimp fabrics Oleksandr Vorobiov 1, Dr. Th. Bischoff 1, Dr. A. Tulke 1 1 FTA Forschungsgesellschaft für Textiltechnik mbh 1 Introduction Noncrimp fabrics (NCFs) are
More informationID1160 REALTIME DETECTION AND EXPLICIT FINITE ELEMENT SIMULATION OF DELAMINATION IN COMPOSITE LAMINATES UNDER IMPACT LOADING
ID116 REALTIME DETECTION AND EXPLICIT FINITE ELEMENT SIMULATION OF DELAMINATION IN COMPOSITE LAMINATES UNDER IMPACT LOADING K. Minnaar and M. Zhou = School of Mechanical Engineering Georgia Institute
More informationPassive Damping Characteristics of Carbon Epoxy Composite Plates
Journal of aterials Science and Engineering A 6 (12) (2016) 3542 doi: 10.17265/21616213/2016.12.005 D DAVID PUBLISHIG Passive Damping Characteristics of Carbon Epoxy Composite Plates Dileep Kumar K
More informationFinite Element Analysis of Composite Laminate By Using ABDH Matrix(Stiffness Matrix)
Finite Element Analysis of Composite Laminate By Using ABDH Matrix(Stiffness Matrix) Nikhil J. Chaudhari 1 Post Graduate Student Department of Mechanical Engineering Veermata Jijabai Technological Institute
More information*MAT_PAPER  a new orthotropic elastoplastic model for paper materials
*MAT_PAPER  a new orthotropic elastoplastic model for paper materials Jesper Karlsson, Dynamore Nordic Mikael Schill, Dynamore Nordic Johan Tryding, Tetra Pak *MAT_PAPER (*MAT_274) A new orthotropic elastoplastic
More informationDELAMINATION CONTROL IN COMPOSITE BEAMS USING PIEZOELECTRIC ACTUATORS
DELAMINATION CONTROL IN COMPOSITE BEAMS USING PIEZOELECTRIC ACTUATORS L Iannucci 1, M S I Shaik Dawood 1,2,3, E Greenhalgh 1 and A K Ariffin 3 1 Aeronautics Department, Imperial College London, South Kensington
More informationIntroduction to Engineering Materials ENGR2000. Dr. Coates
Introduction to Engineering Materials ENGR2 Chapter 6: Mechanical Properties of Metals Dr. Coates 6.2 Concepts of Stress and Strain tension compression shear torsion Tension Tests The specimen is deformed
More informationComposite Laminate Modeling
omposite Laminate Modeling White Paper for Femap and NX Nastran Users Venkata Bheemreddy, Ph.D., Senior Staff Mechanical Engineer Adrian Jensen, PE, Senior Staff Mechanical Engineer WHAT THIS WHITE PAPER
More informationCHEMC2410: Materials Science from Microstructures to Properties Composites: basic principles
CHEMC2410: Materials Science from Microstructures to Properties Composites: basic principles Mark Hughes 14 th March 2017 Today s learning outcomes To understand the role of reinforcement, matrix and
More informationTHREE DIMENSIONAL STRESS ANALYSIS OF THE T BOLT JOINT
THREE DIMENSIONAL STRESS ANALYSIS OF THE T BOLT JOINT Víctor Martínez 1, Alfredo Güemes 2, Norbert Blanco 1, Josep Costa 1 1 Escola Politècnica Superior. Universitat de Girona. Girona, Spain (17071) 2
More informationDEVELOPMENT OF A CONTINUUM PLASTICITY MODEL FOR THE COMMERCIAL FINITE ELEMENT CODE ABAQUS
DEVELOPMENT OF A CONTINUUM PLASTICITY MODEL FOR THE COMMERCIAL FINITE ELEMENT CODE ABAQUS Mohsen Safaei, Wim De Waele Ghent University, Laboratory Soete, Belgium Abstract The present work relates to the
More informationExample3. Title. Description. Cylindrical Hole in an Infinite MohrCoulomb Medium
Example3 Title Cylindrical Hole in an Infinite MohrCoulomb Medium Description The problem concerns the determination of stresses and displacements for the case of a cylindrical hole in an infinite elastoplastic
More informationGeneric Strategies to Implement Material Grading in Finite Element Methods for Isotropic and Anisotropic Materials
University of Nebraska  Lincoln DigitalCommons@University of Nebraska  Lincoln Engineering Mechanics Dissertations & Theses Mechanical & Materials Engineering, Department of Winter 1292011 Generic
More informationChapter 7. Highlights:
Chapter 7 Highlights: 1. Understand the basic concepts of engineering stress and strain, yield strength, tensile strength, Young's(elastic) modulus, ductility, toughness, resilience, true stress and true
More informationUniversity of Bristol  Explore Bristol Research. Early version, also known as preprint
Hallett, S. R., & Wisnom, M. R. (2006). Numerical investigation of progressive damage and the effect of layup in notched tensile tests. Journal of Composite Materials, 40 (14), 12291245. DOI: 10.1177/0021998305057432
More informationLectures on. Constitutive Modelling of Arteries. Ray Ogden
Lectures on Constitutive Modelling of Arteries Ray Ogden University of Aberdeen Xi an Jiaotong University April 2011 Overview of the Ingredients of Continuum Mechanics needed in Soft Tissue Biomechanics
More informationSIMPLIFIED MODELING OF THINWALLED TUBES WITH OCTAGONAL CROSS SECTION AXIAL CRUSHING. Authors and Correspondance: Abstract:
SIMPLIFIED MODELING OF THINWALLED TUBES WITH OCTAGONAL CROSS SECTION AXIAL CRUSHING Authors and Correspondance: Yucheng Liu, Michael L. Day Department of Mechanical Engineering University of Louisville
More informationA FINITE ELEMENT MODEL FOR THE ANALYSIS OF DELAMINATIONS IN FRP SHELLS
TRENDS IN COMPUTATIONAL STRUCTURAL MECHANICS W.A. Wall, K.U. Bletzinger and K. Schweizerhof (Eds.) c CIMNE, Barcelona, Spain 2001 A FINITE ELEMENT MODEL FOR THE ANALYSIS OF DELAMINATIONS IN FRP SHELLS
More informationEFFECT OF LAMINATION ANGLE AND THICKNESS ON ANALYSIS OF COMPOSITE PLATE UNDER THERMO MECHANICAL LOADING
Journal of MECHANICAL ENGINEERING Strojnícky časopis, VOL 67 (217), NO 1, 522 EFFECT OF LAMINATION ANGLE AND THICKNESS ON ANALYSIS OF COMPOSITE PLATE UNDER THERMO MECHANICAL LOADING Arnab Choudhury 1,
More informationEXPERIMENTAL CHARACTERIZATION AND COHESIVE LAWS FOR DELAMINATION OF OFFAXIS GFRP LAMINATES
20 th International Conference on Composite Materials Copenhagen, 1924 th July 2015 EXPERIMENTAL CHARACTERIZATION AND COHESIVE LAWS FOR DELAMINATION OF OFFAXIS GFRP LAMINATES Esben Lindgaard 1 and Brian
More informationADVANCES IN THE PROGRESSIVE DAMAGE ANALYSIS OF COMPOSITES
NAFEMS WORLD CONGRESS 13, SALZBURG, AUSTRIA ADVANCES IN THE PROGRESSIVE DAMAGE ANALYSIS OF M. Bruyneel, J.P. Delsemme, P. Jetteur (LMS Samtech, Belgium); A.C. Goupil (ISMANS, France). Dr. Ir. M. Bruyneel,
More informationCHARACTERIZATION, ANALYSIS AND PREDICTION OF DELAMINATION IN COMPOSITES USING FRACTURE MECHANICS
Oral Reference Number: ICF100942OR CHARACTERIZATION, ANALYSIS AND PREDICTION OF DELAMINATION IN COMPOSITES USING FRACTURE MECHANICS T. Kevin O Brien U.S. Army Research Laboratory Vehicle Technology Directorate
More informationAfter lecture 16 you should be able to
Lecture 16: Design of paper and board packaging Advanced concepts: FEM, Fracture Mechanics After lecture 16 you should be able to describe the finite element method and its use for paper based industry
More informationMaterials and Structures. Indian Institute of Technology Kanpur
Introduction to Composite Materials and Structures Nachiketa Tiwari Indian Institute of Technology Kanpur Lecture 15 Behavior of Unidirectional Composites Lecture Overview Mt Material ilaxes in unidirectional
More informationExperimental and theoretical characterization of Li 2 TiO 3 and Li 4 SiO 4 pebbles
Experimental and theoretical characterization of Li 2 TiO 3 and Li 4 SiO 4 s D. Aquaro 1 N. Zaccari ABSTRACT Dipartimento di Ingegneria Meccanica Nucleare e della Produzione University of Pisa (Italy)
More informationCOMPUTER AIDED DESIGN IN CASE OF THE LAMINATED COMPOSITE MATERIALS
6 th International Conference Computational Mechanics and Virtual Engineering COMEC 15 1516 October 15, Braşov, Romania COMPUER AIDED DESIGN IN CASE OF HE LAMINAED COMPOSIE MAERIALS Camelia Cerbu ransilvania
More informationInterlaminar fracture characterization in composite materials by using acoustic emission
5th International Symposium on NDT in Aerospace, 1315th November 2013, Singapore Interlaminar fracture characterization in composite materials by using acoustic emission Ian SILVERSIDES 1, Ahmed MASLOUHI
More informationDESIGN OF COMPOSITE LAMINATED STRUCTURES BY POLAR METHOD AND TOPOLOGY OPTIMISATION
DESIGN OF COMPOSIE LAMINAED SUCUES BY POLA MEOD AND OPOLOGY OPIMISAION A. Jibawy,,3, C. Julien,,3, B. Desmorat,,4, (*), A. Vincenti UPMC Univ Paris 6, UM 79, Institut Jean Le ond d Alembert B.P. 6 4, place
More informationMATERIAL MECHANICS, SE2126 COMPUTER LAB 4 MICRO MECHANICS. E E v E E E E E v E E + + = m f f. f f
MATRIAL MCHANICS, S226 COMPUTR LAB 4 MICRO MCHANICS 2 2 2 f m f f m T m f m f f m v v + + = + PART A SPHRICAL PARTICL INCLUSION Consider a solid granular material, a so called particle composite, shown
More informationPressure Vessels Stresses Under Combined Loads Yield Criteria for Ductile Materials and Fracture Criteria for Brittle Materials
Pressure Vessels Stresses Under Combined Loads Yield Criteria for Ductile Materials and Fracture Criteria for Brittle Materials Pressure Vessels: In the previous lectures we have discussed elements subjected
More informationSUBSURFACE DAMAGE LOCATION AND IDENTIFICATION USING INFRARED TECHNIQUES
SUBSURFACE DAMAGE LOCATION AND IDENTIFICATION USING INFRARED TECHNIQUES T.R. Emery 1, J. M. DulieuBarton 1, P.R. Cunningham 2 1 University of Southampton, School of Engineering Sciences, SO17 1BJ, UK
More informationAE3610 Experiments in Fluid and Solid Mechanics TRANSIENT MEASUREMENTS OF HOOP STRESSES FOR A THINWALL PRESSURE VESSEL
Objective AE3610 Experiments in Fluid and Solid Mechanics TRANSIENT MEASUREMENTS OF OOP STRESSES FOR A TINWA PRESSURE VESSE This experiment will allow you to investigate hoop and axial stress/strain relations
More informationBone Tissue Mechanics
Bone Tissue Mechanics João Folgado Paulo R. Fernandes Instituto Superior Técnico, 2016 PART 1 and 2 Introduction The objective of this course is to study basic concepts on hard tissue mechanics. Hard tissue
More informationThe Frictional Regime
The Frictional Regime Processes in Structural Geology & Tectonics Ben van der Pluijm WW Norton+Authors, unless noted otherwise 1/25/2016 10:08 AM We Discuss The Frictional Regime Processes of Brittle Deformation
More informationNonconventional Glass fiber NCF composites with thermoset and thermoplastic matrices. F Talence, France Le Cheylard, France
20 th International Conference on Composite Materials Copenhagen, 1924th July 2015 Nonconventional Glass fiber NCF composites with thermoset and thermoplastic matrices. Thierry Lorriot 1, Jalal El Yagoubi
More informationPredicting Fatigue Life with ANSYS Workbench
Predicting Fatigue Life with ANSYS Workbench How To Design Products That Meet Their Intended Design Life Requirements Raymond L. Browell, P. E. Product Manager New Technologies ANSYS, Inc. Al Hancq Development
More informationDirect Comparison of Anisotropic Damage Mechanics to Fracture Mechanics of Explicit Cracks
Direct Comparison of Anisotropic Damage Mechanics to Fracture Mechanics of Explicit Cracks John A. Nairn Wood Science and Engineering, Oregon State University, Corvallis, OR 97330, USA Tel: +15417374265
More informationSANDWICH COMPOSITE BEAMS for STRUCTURAL APPLICATIONS
SANDWICH COMPOSITE BEAMS for STRUCTURAL APPLICATIONS de Aguiar, José M., josemaguiar@gmail.com Faculdade de Tecnologia de São Paulo, FATECSP Centro Estadual de Educação Tecnológica Paula Souza. CEETEPS
More informationOutline. TensileTest Specimen and Machine. StressStrain Curve. Review of Mechanical Properties. Mechanical Behaviour
TensileTest Specimen and Machine Review of Mechanical Properties Outline Tensile test True stress  true strain (flow curve) mechanical properties:  Resilience  Ductility  Toughness  Hardness A standard
More informationIMPACT ON LAMINATED COMPOSITE PLATES: COMPARISON OF TEST AND SIMULATION RESULTS OBTAINED WITH LMS SAMTECH SAMCEF
V ECCOMAS Thematic Conference on the Mechanical Response of Composites COMPOSITES 015 S.R. Hallett and J.J.C. Remmers (Editors) IMPACT ON LAMINATED COMPOSITE PLATES: COMPARISON OF TEST AND SIMULATION RESULTS
More informationAim of the study Experimental determination of mechanical parameters Local buckling (wrinkling) Failure maps Optimization of sandwich panels
METNET Workshop October 1112, 2009, Poznań, Poland Experimental and numerical analysis of sandwich metal panels Zbigniew Pozorski, Monika ChudaKowalska, Robert Studziński, Andrzej Garstecki Poznan University
More informationUNIT 1 STRESS STRAIN AND DEFORMATION OF SOLIDS, STATES OF STRESS 1. Define stress. When an external force acts on a body, it undergoes deformation.
UNIT 1 STRESS STRAIN AND DEFORMATION OF SOLIDS, STATES OF STRESS 1. Define stress. When an external force acts on a body, it undergoes deformation. At the same time the body resists deformation. The magnitude
More informationOn matrixdriven failure in unidirectional NCF composites
THESIS FOR THE DEGREE OF LICENTIATE OF ENGINEERING IN SOLID AND STRUCTURAL MECHANICS On matrixdriven failure in unidirectional NCF composites A theoretical and experimental study DENNIS WILHELMSSON Department
More informationBasic Energy Principles in Stiffness Analysis
Basic Energy Principles in Stiffness Analysis StressStrain Relations The application of any theory requires knowledge of the physical properties of the material(s) comprising the structure. We are limiting
More informationDon Robbins, Andrew Morrison, Rick Dalgarno Autodesk, Inc., Laramie, Wyoming. Abstract
PROGRESSIVE FAILURE SIMULATION OF ASMANUFACTURED SHORT FIBER FILLED INJECTION MOLDED PARTS: VALIDATION FOR COMPLEX GEOMETRIES AND COMBINED LOAD CONDITIONS Don Robbins, Andrew Morrison, Rick Dalgarno Autodesk,
More informationChapter 2 A Continuum Damage Model Based on Experiments and Numerical Simulations A Review
Chapter 2 A Continuum Damage Model Based on Experiments and Numerical Simulations A Review Michael Brünig Abstract The paper summarizes the author s activities in the field of damage mechanics. In this
More informationPLAT DAN CANGKANG (TKS 4219)
PLAT DAN CANGKANG (TKS 4219) SESI I: PLATES Dr.Eng. Achfas Zacoeb Dept. of Civil Engineering Brawijaya University INTRODUCTION Plates are straight, plane, twodimensional structural components of which
More informationASSESSMENT OF DYNAMICALLY LOADED CRACKS IN FILLETS
ASSESSMENT OF DNAMICALL LOADED CRACKS IN FILLETS Uwe Zencker, Linan Qiao, Bernhard Droste Federal Institute for Materials Research and Testing (BAM) 12200 Berlin, Germany email: zencker@web.de Abstract
More information